COMPARATIVE STUDY OF MECHANICAL PROPERTIES OF 316L STAINLESS STEEL BETWEEN TRADITIONAL PRODUCTION METHODS AND SELECTIVE LASER MELTING
A thesis presented to the faculty of the Graduate School of Western Carolina University in partial fulfillment of the requirements for the degree of Master of Science in Technology.
Alton Dale Lackey
Advisor: Wes Stone, Ph.D.
Associate Professor, Department of Engineering & Technology Committee:
Sudhir Kaul, Ph.D., Department of Engineering & Technology Aaron Ball, Ed.D. Department of Engineering & Technology
ii TABLE OF CONTENTS LIST OF TABLES ... iv LIST OF FIGURES ...v LIST OF EQUATIONS... vi ABSTRACT ... vii
Chapter One: INTRODUCTION ...1
Additive Manufacturing ...4
History of Additive Manufacturing ...5
Consolidation Methods ...6
Build Strategy/Orientations of Parts ...6
Subtractive Manufacturing ...7
Mechanical Properties ...8
Provisions of the Study ... 10
Chapter Two: LITERATURE REVIEW ... 16
Additive Manufacturing ... 16
SLM ... 16
SLM/EOS System ... 17
SLS vs. SLM, Partial vs. Full Melting ... 17
316L Stainless ... 19
Material Specifics ... 20
Microstructure and Grain Structure from SLM Process ... 23
Effects of Various Orientations ... 25
EOS Machine Specifics ... 29
Tensile Properties/Test ... 31
Stress Risers ... 31
Standard for Tensile Testing Metals ... 32
Chapter Three: METHODOLOGY ... 34
Preliminary Procedures ... 34
SLM Preparation ... 35
Part position and Support Structure ... 35
Machine preparation ... 39
Preparation of Printed Pieces ... 40
Experimental Procedures ... 44
Tensile Testing... 44
Chapter Four: RESULTS ... 47
Chapter Five: ANALYSIS AND CONCLUSIONS ... 58
Analysis of Findings for Tensile Testing Comparison Experiment ... 58
Expected Results ... 58
Stress-Strain Graph ... 59
Material Composition... 61
Statistical Analysis of Results ... 62
Boxplots of Each Mechanical Property ... 62
Comparison F-Tests and T-Tests ... 65
Additional Statistical Analysis ... 68
Conclusions ... 73
REFERENCES ... 76
Part Summary Tables... 78
Analysis of Variance Using F-Test ... 84
F-Tests for Calculated Yield Strength ... 84
F-Tests for Extensometer Yield Strength ... 87
F-Tests for UTS ... 88
F-Tests for Extensometer Young’s Modulus ... 90
Comparison of Sample Means Using T-Test ... 92
T-Tests for Calculated Yield Strength ... 92
T-Tests for Extensometer Yield Strength ... 95
T-Tests for UTS... 96
T-Tests for Extensometer Young’s Modulus ... 99
Stress – Strain Graphs... 102
Stress – Strain Graphs of SLM Edge Parts ... 103
Stress – Strain Graphs of SLM Flat Parts ... 113
Stress – Strain Graphs of Purchased Parts ... 126
Boxplots of Mechanical Properties ... 136
Normal Probability Plots of Mechanical Properties ... 138
Minitab Statistical Analysis results ... 140
Minitab GLM Results ... 140
LIST OF TABLES
Table 1-1: EOS Metal Materials ...7
Table 2-1: Expected Chemical Composition of EOS 316L Stainless Steel Parts ... 19
Table 2-2: Expected Chemical Composition of Purchased 316L Stainless Steel Parts ... 19
Table 4-1: Collected Means of mechanical properties of specimen groups... 49
Table 4-2: F-Test Summary Results Table ... 50
Table 4-3: T-Test Results Summary Table ... 51
Table 4-4: Ordered Extensometer Yield Strength Data and Calculated Part Difference ... 55
Table 4-5: f-Test Comparing Calculated Part Differences ... 56
Table 4-6: t-Test Comparing Calculated Part Differences ... 56
Table 4-7: Mean and Standard Deviation used for Monte Carlo Method ... 56
Table 4-8: f-Test Comparing Part Differences using Monte Carlo Method ... 57
Table 4-9: t-Test Comparing Part Differences using Monte Carlo Method... 57
Table 5-1: Measured Material Composition of EOS 316L Stainless Steel ... 62
LIST OF FIGURES
Figure 1-1: Example of Typical Stress Strain Curve ... 10
Figure 2-1: Laser-based powder consolidation mechanisms... 17
Figure 2-2: TGM inducing residual stress ... 22
Figure 2-3: Balling characteristics when oxygen=0.1% ... 24
Figure 2-4: Orthogonal Orientation Notation ... 25
Figure 2-5: Example of Symmetry Abbreviation of Orthogonal Orientation Notation ... 26
Figure 2-6: Representation of various orientations of tensile samples with respect to building direction (oz) ... 28
Figure 2-7: Tensile specimen containing a circular hole stress concentration ... 32
Figure 3-1: Rectangular Tension Test Specimens ... 34
Figure 3-2: Flat oriented specimen showing support structure ... 35
Figure 3-3: Flat test specimen with stress concentration and support structure ... 36
Figure 3-4: Edge oriented test specimen showing supported stress concentration... 37
Figure 3-5: Edge oriented test specimen build without stress concentration supports ... 37
Figure 3-6: Build Plat Layout ... 38
Figure 3-7: Finished SLM parts encased in excess powdered metal ... 41
Figure 3-8: Support Material Tooth Structure ... 42
Figure 3-9: Fixture for repeatability of drilling in specimens ... 43
Figure 3-10: Instron Part Test Set-up ... 45
Figure 4-1: Example of Stress-Strain Diagram using data from Purchased Solid Part 1-1 ... 48
Figure 4-2: Boxplot of Calculated Yield Strength ... 49
Figure 4-3: Normal Probability Plot of Extensometer Yield Strength for Purchased Solid Parts . 52 Figure 4-4: Residual Plots created by the GLM in Minitab ... 53
LIST OF EQUATIONS
Equation 1-1 ...8 Equation 1-2 ...9 Equation 1-3 ...9
COMPARATIVE STUDY OF MECHANICAL PROPERTIES OF 316L STAINLESS STEEL BETWEEN TRADITIONAL PRODUCTION METHODS AND SELECTIVE LASER
Alton Dale Lackey, M.S.T
Western Carolina University (April 2016)
Additive manufacturing, also known as 3D printing, is a technology which has recently seen expanding use, as well as expansion of the materials and methods able to be used. This thesis looks at the comparison of mechanical properties of 316L stainless steel manufactured by both traditional methods and selective laser melting found by tensile testing. The traditional method used here involved cold rolled 316L steel being machined to the desired part geometry. Selective laser melting used additive manufacturing to produce the parts from powdered 316L stainless steel, doing so in two different build orientations, flat and on edge with regards to the build plate. Solid test specimens, as well as specimens containing a circular stress concentration in the center of the parts, were manufactured and tensile tested. The tensile tests of the specimens were used to find the mechanical properties of the material; including yield strength, ultimate tensile strength (UTS), and Young’s modulus of elasticity; where statistical analyses were performed to determine if the different manufacturing processes caused significant differences in the
mechanical properties of the material. These analysis consisting of f-tests, to test for variance, and t-test, testing for significant difference of means. Through this study it was found that there were statistically significant differences existing between the mechanical properties of selective
laser melting, and its orientations, and cold roll forming of production of parts. Even with a statistical difference, it was found that the results were reasonably close between flat oriented SLM parts and purchased parts. So it can be concluded that, with regards to strength, SLM methods produce parts similar to traditional production methods.
CHAPTER ONE: INTRODUCTION
This research focuses on the impact of using the Selective Laser Melting (SLM) process to include part features in 316L stainless steel, while comparing the effect varying part orientations and manufacturing processes has on material properties. Using both traditional methods, in this case cold roll forming, and advanced production methods, SLM, two geometries were produced for tensile testing, and the results statistically analyzed. The two geometries are that of tensile testing specimens, one with a solid geometry, and another containing a circular stress
concentration. For the purposes of this research, the EOS M290 SLM system was operated using predetermined process parameters provided through EOS, including predetermined support structure geometry. The tensile testing was completed with accordance of the ASTM E8 standard test methods for tension testing of metallic materials, which in turn allowed the mechanical properties of the various production methods to be determined.
The objective of this research was to determine, through statistical analysis, if the SLM process is able to produce parts with similar mechanical properties as parts produced using traditional methods. For this experiment the SLM process, and its various build orientations, will be compared with annealed cold rolled 316L stainless steel. The research specifically looked into how each production method handles the addition of stress concentrations in tensile testing specimen, while looking in the area of part strength, in detail in yield strength. It was made certain that each production methods produced the geometries to specific dimensions, including similarly sized stress concentrations. The cold rolled specimens were purchased without prior testing, so that the specimens from each production method would receive tensile testing within
the same environment, using the same equipment. Within each mechanical properties found for the production methods, comparisons were made to match corresponding geometries during statistical analysis. Being an important mechanical property of the material, when being used in part production, the yield strength of the specimens was utilized in further statistical analysis to determine how different production methods responded when containing a stress concentration.
With regards to the comparison of various production methods of tensile testing specimens, it was expected that testing results would reflect similarly from each method. Each mechanical property found; yield strength, Young’s modulus of elasticity, ultimate tensile strength (UTS); could then be used in the comparison of the various production methods. These comparisons of mechanical properties comprising of the following:
SLM Edge Solid vs. SLM Flat Solid
SLM Edge Solid vs. Purchased Solid
SLM Flat Solid vs. Purchased Solid
SLM Edge with Hole vs. SLM Flat with Hole
SLM Edge with Hole vs. Purchased with Hole
SLM Flat with Hole vs. Purchased with Hole
These comparisons were to be used in the statistical analysis of the production methods to determine if a significant difference exists in each mechanical property. The first analysis to be completed is an analysis of variance. For this an f-test will be used in each comparison for each property. The f-tests will contain a null and alternate hypothesis to determining the result of the variance analysis. This is statistically expressed in the null hypothesis:
Accepting the null hypothesis given here would show a result stating the variances of the two production methods are assumed equal. If the result states the null hypothesis is rejected, then an alternate hypothesis must be accepted. The alternate hypothesis for these f-tests would appear as follows:
This alternate hypothesis states that the results of the analysis of variance show the two variances are assumed to be unequal. The f-tests are only to be used in analyzing the variance of the
comparisons, another analysis method must be used to compare the means of the production methods.
Following the analysis of variance, a comparison of the means should be used. This is done using t-tests, which use the results of the f-tests previously ran, where the t-test will assume equal or unequal variances for the comparisons. Just as with the f-tests, a hypothesis must be created before testing, in this case the null is as follows:
Where for t-tests, this null hypothesis, if failed to reject, states the means of the mechanical properties being compared are not significantly different from one another. If the null is rejected, then the alternate hypothesis is then accepted. This alternate hypothesis is as follows:
The alternate hypothesis shown here, if the null hypothesis is rejected, states that the two means of the production methods being compared are significantly different. Again, as stated, these null and alternate hypotheses for both the f-tests and t-tests are to be applied to each comparison of production method shown.
An ANOVA allows the analysis of the differences between various group means, and thus may be used to make multiple comparisons with one method, but is otherwise similar to t-tests as it compares group means. Again for the ANOVA a hypothesis must be formed, the null hypothesis is stated as follows:
Which states that all sample means (i) are statistically equal to one another. As in other statistical analysis methods, an alternate hypothesis is also needed and is given here:
Which states that at least one sample mean is significantly different from another, thus stating the means are unequal. After performing an ANOVA, if the results do show a significant difference is present, it is possible to perform a post-hoc test. This test is used to determine where the differences occurred between groups. This test also uses the results of a test of variance,
assuming either equal or unequal variances. This result determines which type of post hoc test is used, where equal variances utilize the Tukey post hoc test, and unequal variances use a Games-Howell post hoc test. The results of both these post hoc tests produce a chart showing intervals of each comparison made, where the intervals may be used to determine significance of the
As manufacturing processes continue to improve and develop, the demand for faster and less expensive manufacturing processes have allowed for a number of Rapid Prototyping (RP) processes to be developed. RP technology is unconstrained by the limitations of specially designed tooling and fixturing. Therefore, almost any geometry with variation in size and complexity can be produced to a high degree of accuracy (Simchi & Asgharzadeh, 2004). RP
techniques are capable of manufacturing complex 3D geometries by using Additive
Manufacturing (AM). Rather than removing material from a stock until a desired geometry is met, as found in Subtractive Manufacturing (SM), material is added in specifically shaped layers to build up the geometry. Each successive layer of material is adhered to the previous layer by some form of controlled heat exposure, depending on the method used. Initially AM techniques were used to create prototypes or any low quantity amount of parts. Though currently the use of AM is not limited to prototyping or as a temporary stage in the design but rather includes many applications of the technology, including, modeling, pattern-making, tool-making, and the production of end-use parts in large quantities (Banther, 2009) (Kruth, et al., 2010).
With the EOS Parameter Sets, the system manufactures parts with standardized Part Property Profiles (PPPs) for a broad range of applications (EOS e-Manufacturing Solutions, 2014b). Each material is assigned one or more parameter sets with corresponding PPPs. These PPPs typically include the following groups of properties:
Geometric properties such as minimum wall thickness and surface roughness
Mechanical properties such as tensile strength, yield strength, elongation at break, modulus of elasticity and hardness, and where applicable dynamic fatigue life
Thermal attributes such as thermal conductivity, specific heat capacity and thermal expansion coefficient
History of Additive Manufacturing
Varying methods of AM have been recorded as early as 1890, where a layering method was used to build up topographical maps. At the time, each layer was cut, shaped, and laid by hand. Though not an extremely precise method, it accomplished what was needed at the time (Bourell, Beaman, Jr., Leu, & Rosen, 2009). In 1972 another process was developed for
manufacturing maps that involved selectively exposing photo-hardening material to a heat source. Each layer of the material only harden where the heat was applied allowing for an improved, more automated, process. In 1979 the earliest description of a powder laser sintering process was proposed in a patent. Then 1981 A. J. Herbert described the development of a system that directs a UV laser beam to a photopolymer layer by means of mirror system on an x-y plotter.
As AM technology has developed over time, the use or goals for the parts have also changed, for example different materials are demanded for various uses. This in turn then
requires a new method or process depending on the material. Kruth (2007) gives examples of the most popular layered manufacturing techniques, being: photo-polymerization, Stereolithography (SLA and its derivatives), ink-jet printing (IJP), 3D printing (3DP), Fused Deposition Modelling (FDM), Selective Laser Sintering or Melting (SLS/SLM and Electron Beam Melting) (Kruth, Levy, Klocke, & Childs, 2007). Within many of these methods are specific binding mechanisms, though this study will focus on the outcome of full melting SLM manufacturing methods,
specifically using the e-Manufacturing Solutions EOS M290 Metal Additive Manufacturing System, housed within The Kimmel School of Western Carolina University.
Build Strategy/Orientations of Parts
As a greater number and better performing systems using SLM are being developed, the number of available materials also increases. As stated before the SLM process is able to use various powdered materials in polymers, ceramics and metals. EOS e-Manufacturing solutions produces systems for both SLM of polymers and metals, with multiple systems for each material type. Note that each system is setup for either polymers or metals. A list of currently available
powdered metals from EOS can be found in Table 1-1. This research will be done using the 316L Stainless Steel made by EOS.
Subtractive manufacturing (SM), as stated, is the removal of material from a stock to produce a desired 3D geometry. SM requires the use of a computer numerical control (CNC) machine, typically found in the form of mills, lathes, grinders, or water-jet cutters. These machines have improved greatly over time, but are still limited in capability by the available tooling and methods. A significant difference between SM and AM is the process by which the
material is subject to. While SM removes from already solidified stock material, AM works by solidifying loose material to the preferred shape. The loose material can usually be found in the form of powder. For the purpose of this research, test specimens were purchased from Lab
Composition Trade Name
Maraging Steel EOS MaragingSteel MS1
EOS StainlessSteel GP1
EOS StainlessSteel CX
EOS StainlessSteel 316L
EOS StainlessSteel PH1
EOS NickelAlloy IN718
EOS NickelAlloy IN625
EOS Nickel Alloy HX
EOS CobaltChrome MP1
EOS CobaltChrome SP2
Titanium EOS Titanium Ti64
Aluminium EOS Aluminium AlSi10Mg EOS Metal Materials
Table 1-1: EOS Metal Materials (EOS e-Manufacturing Solutions, 2013)
Testing Incorporated, where cold rolled 316L stainless steel was machined to the correct dimensional geometry. The process of cold rolling is performed close to normal room
temperature and uses pressure to change the size of the material being processed. In the case of these parts, the material was cold rolled into bar stock which was then used in milling the parts to the desired dimensions.
Mechanical Properties Tensile Testing
This research will focus on the comparison of mechanical properties of 316L stainless steel between two manufacturing methods, SLM and subtractive manufacturing, in this case milling. The mechanical properties of these materials will be determined by tensile testing. A tensile test, also known as tension test, is performed by pulling on a material, usually until failure. By doing this test a tensile profile will be formed in a curve showing how the material reacted to the forces being applied (Instron, n.d.). Data can then be interpreted from the tensile profile taken from the material. This experiment will be looking into; stress, strain, yield stress, ultimate tensile stress, and Young’s modulus of elasticity. Stress is the internal resistance of a material to distorting effects of an external force or load. The calculation for stress can be found in Eq. 3.1, where σ equals stress, F is the force being applied, and A is the cross-sectional area of the specimen. The resulting unit for stress is MPa.
𝜎 = 𝐹/𝐴 Equation 1-1
Strain is defined as the deformation of a solid due to stress. This can be seen as the elongation during tensile testing. Strain is calculated using the equation Eq. 3.2, where is the unit-less measure of strain, Δl is the change in length, and l0 is initial length.
𝜀 = ∆𝑙/𝑙0 Equation 1-2
Young’s modulus of elasticity is a measure of stiffness of an elastic material, and is used to describe the elastic properties of objects when they are stretched or compressed. The equation for Young’s modulus can be found in Eq 3.3. This elastic modulus is a ratio of stress and strain, and once known can be used to predict the elongation or compression of an object where the stress is less than the yield strength of the material, otherwise known as the elastic region. Young’s modulus is represented by E and units MPa.
𝐸 = 𝜎 𝜀⁄ Equation 1-3
The Young’s modulus is only applicable to materials when they remain in the elastic region during testing. This elastic region is the area before the yield strength of a material. The positioning of the Young’s modulus can be seen in Figure 1-1. As can be seen, the Young’s modulus appears parallel to the beginning part of the elastic region of the stress-strain curve, though it is offset in the strain by 0.2%. Where the Young’s modulus intersects with the stress-strain curve is the yield strength of the material, or the end of the elastic region.
Also visible in the example stress-strain curve is the ultimate tensile strength (UTS). This is a value found by locating the maximum amount of stress within the stress-strain curve, as indicated in the diagram at the peak of the curve.
Provisions of the Study
It has been stated, this study will encompass various production methods for tensile testing specimens. These production methods specifically include the SM method of machining of cold rolled bar stock of 316L stainless steel, to a dimensional geometry described by ASTM E8. The other method entails using the AM method of SLM manufacturing of 316L powdered metal, provided by EOS e-manufacturing, producing the parts to the same dimensional geometry. Within the SLM process two build orientations will be included. These two build orientations involve the part being in a flat orientation, which is parallel to the build surface, and an edge orientation, where the part is perpendicular to the build surface. For both production methods, the same 316L stainless steel was used so the results would reflect the production methods and not variations in materials. A parameter set predetermined and provided by EOS
e-Figure 1-1: Example of Typical Stress Strain Curve (IHS Engineering 316, 2006)
manufacturing was used in each part production. These parameters included machine parameters as well as support structure design and dimensions.
The preparations of the stress concentrations vary between the different production methods. For the flat oriented SLM produced parts, no preparation or post processing of the actual stress concentrations are needed. The edge oriented SLM produced parts, support structure was needed within the stress concentration and thus was required to be removed before testing, which was done by use of a metal file. A stress concentration could not be placed in the part during the production using traditional methods. The stress concentration was placed in these parts by use of a milling machine to drill the correct size hole into the parts, which was
consistently done for each traditional production part which required the stress concentration. The tensile testing of this research was done in accordance with the ASTM E8 standard of tensile testing metals. The requirements of testing set forth by this standard were used for testing of all test specimens. The entirety of tensile testing was performed using the Instron 5960 series dual column testing system. Also the testing of parts for this research was limited to tensile testing of the parts, as the desired mechanical properties can be found from tensile testing. These mechanical properties were limited to yield strength, UTS and Young’s modulus, for this study.
As AM production methods become more commonly used, it is important to know the potentiality of what the method can produce. This includes but is not limited to knowing the effects SLM production has on the mechanical properties of a material when compared to traditional methods of production, when is explored in this research. This study also investigates the comparison of the methods when including a part geometry in tensile testing specimens. Moving forward in new technologies and production methods it is necessary to know the capabilities of the methods used.
So as we see here, this research will be looking into the comparison of various
manufacturing methods, with regards to mechanical properties of the parts, and will be achieved by performing the following:
All production methods will use 316L stainless steel
The SLM process will include two build orientations, edge and flat
All the SLM produced and purchased parts will include two geometries, with and without the same size stress concentrations
Tensile testing will be performed, using the same test setup for each production method
Mechanical properties, yield strength, UTS, and Young’s modulus will be extracted from the tensile testing results
Comparisons of the production methods will be made for each mechanical property
Statistical analyses of these comparisons within each mechanical property will be made and conclude in either a significant difference being present or absent Following these procedure, this research will determine whether using SLM production methods to produce parts, both with and without stress concentrations, or traditional manufacturing of parts containing the same geometry will result in similar or varying mechanical properties.
Additive Manufacturing (AM) – a process of joining materials to make objects from 3D model data, usually layer upon layer, as opposed to subtractive manufacturing methodologies. Arbitrarily oriented minimum bounding box – of a part, the minimum perimeter cuboid that can
span the maximum extents of the points on the surface of a 3D part calculated without any constraints on the resulting orientation of the box.
Build Platform (Build Plate) – of a machine, any base which provides a surface upon which the build is started and supported throughout the build process.
Build Surface – area where material is added, normally on the last deposited layer which becomes the foundation upon which the next layer is formed.
CAD – Computer-Aided Design. The use of computers for the design of real or virtual objects. CAM – Computer-Aided Manufacturing. Typically refers to systems that use surface data to
drive CNC machines, such as digitally-driven mills and lathes, to produce parts, molds, and dies.
CNC – Computer Numerical Control. Computerized control of machines for manufacturing. Initial Build Orientation – of a part, is the orientation of the part as first placed in the build
volume and becomes the reference for any further part reorientation.
Orthogonal Orientation Notation – of a part’s initial build orientation, may be used when the intended build orientation for a part is such that its arbitrarily oriented minimum bounding box is aligned parallel to the X, Y, and Z axes of the build volume origin, its orientation may be described by listing which axis is parallel to the longest overall dimension of the bounding box first, followed by the axis which is parallel to the second
longest overall dimension of the bounding box second, followed by the axis which is parallel to the third longest overall dimension of the bounding box.
Rapid Prototyping (RP) – additive manufacturing of a design, often iterative, for form, fit, or functional testing, or combination thereof.
Selective Laser Melting (SLM) – a powder bed fusion process used to produce objects from powdered materials using one or more lasers to selectively fuse or melt the particles at the surface, layer by layer, in an enclosed chamber.
STL (STereoLithography) – in additive manufacturing, file format for 3D model data used by machines to build physical parts; STL is the de facto standard interface for additive manufacturing systems.
Stress – in mechanics, the force per unit area on a body that tends to cause it to change shape. Stress is a measure of the internal forces in a body between its particles. These internal forces are a reaction to the external forces applied on the body that cause it to separate, compress or slide.
Subtractive Manufacturing (SM) – making objects by removal of material (for example, milling drilling, grinding, carving, etc.) from a bulk solid to leave a desired shape, as opposed to additive manufacturing.
Ultimate Tensile Strength (UTS) – the capacity of a material or structure to withstand loads tending to elongate.
X axis – of a machine, shall run perpendicular to the Z axis and parallel to the front of the machine.
Y axis – of a machine, shall run perpendicular to the Z and X axes with positive direction defined to make a right hand set of coordinates as specified in ISO 841.
Z axis – of a machine, for processes employing planar layerwise addition of material, shall run normal to the layers. Shall run perpendicular to the X and Y axes with positive direction being vertical to the work area.
CHAPTER TWO: LITERATURE REVIEW
The research presented here discusses the effect various production methods have on material properties. Previously, several studies have been conducted in related areas. The related areas being effects of SLM manufacturing, AM processes involving 316L stainless steel, and part orientation during SLM. At this time no research has been found with regards to
purposefully including part features or stress risers in the SLM process and how it effects material properties.
When looking at the detailed descriptions of the history of AM, it becomes apparent how the various techniques used individually in the past were able to come together and influence the methods used today. The selective heat exposure to materials has been used it many techniques, though in new methods the accuracy of the heat exposure has be greatly increased. The
improvement of these methods also included the use of layerwise scanning of the geometry, where one layer was formed at a time. This improvement in heat exposure accuracy is due to both the advancement in technology, but also a technique which introduced the use of a laser beam controlled by a computer and directed by a set of mirrors. SLM is an AM process which uses many of these techniques, which were developed over time, in one production method.
SLM/EOS System SLS vs. SLM, Partial vs. Full Melting
It can be said that SLS and SLM are similar methods, in that both utilize a computer controlled laser to consolidate layers of metal powder onto previously consolidated layers. The distinction between SLS and SLM is vague and does not cover all types of consolidation, though a more detailed specification of binding mechanisms can be found in Figure 2-1. Looking at these binding mechanisms allows for a better discrepancy to be made between SLS and SLM methods. Solid state sintering (SSS) is a consolidation process which occurs below the materials melting temperature. The material consolidates by forming necks between adjacent powder particles which grow larger over time. This consolidation technique is used primarily with ceramics, as the diffusion rate of atoms in SSS is slow and not feasible for process productivity (Kruth, Levy, Klocke, & Childs, 2007). Liquid phase sintering (LPS) and partial melting include a variety of binding mechanisms in which part of the powder material is melted while other parts remain solid. As some of the material is melted it quickly moves between the remaining solid material, binding the material together. The material that melts to become the binder may not be
Figure 2-1: Laser-based powder consolidation mechanisms (Kruth, Levy, Klocke, & Childs, 2007)
the same as that which remains solid. For example a material containing coated particles could be used in which the coating material has a lower melting temperature which would allow it to solely react to the applied heat. Partial melting can also be used when there is no distinct binding material. In this use the SLS parameters are adjusted to only partially melt the powder particles. LPS and partial melting typically require a post process to produce a fully dense part (Kruth, Levy, Klocke, & Childs, 2007). Full melting, used in SLM, is a major consolidation mechanism often used to achieve fully dense parts without need for any post-process densification. While it has the advantage of no post-processing there are some potential drawbacks that can occur without carful process control. Balling phenomena is a possible SLM defect and can be
detrimental to the forming quality of the parts. Within the balling behavior there are two possible types; an ellipsoidal balls with a dimension of 500 µm and spherical balls with dimension of about 10 µm. The ellipsoidal balls tend to cause problems with quality while the spherical balls are not as significant. Some main disadvantages caused by balling given by Li (2012) are as follows:
1. The balling phenomenon could increase the surface roughness; thus, requiring some post-process such as polishing. While trivial, this could also cause dimensional inaccuracy. 2. A large amount of pores in SLM component tend to form between many discontinuous
metallic balls, which result in a lesser density and thus results in poor mechanical properties.
3. When the balling phenomenon is severe enough there is potential for the balls to hinder the movement of the recoater blade of the layering system. The result is either the part is slightly damaged or scratched, or the recoater blade is stopped completely (Li, Liu, Shi, Wang, & Jiang, 2012).
The materials used in the SLM process begin as very fine powdered metal, with the powder particles ranging in sizes of 5-10 µm. Most manufacturers of SLM systems also produce metal powder mixtures that work best with their system. EOS Stainless Steel 316L is a corrosion resistant iron based alloy which has been optimized especially for processing on EOSINT M290
Material Composition Element Min. Max.
Fe 58.23 73.61 Cr 16.00 18.50 Ni 10.00 15.00 Mo - 3.00 C - 0.08 Mn - 2.00 Cu - 1.00 P - 0.045 S - 0.35 Si - 1.00 N - 0.10 Ti - 0.70
Expected Chemical Properties of Parts
Purchased Stainless Steel 316L Table 2-2: Expected Chemical Composition of Purchased
316L Stainless Steel Parts
Table 2-1: Expected Chemical Composition of EOS 316L Stainless Steel Parts
Material Composition Element Min. Max. Fe Cr 17.00 19.00 Ni 13.00 15.00 Mo 2.25 3.00 C - 0.03 Mn - 2.00 Cu - 0.50 P - 0.025 S - 0.01 Si - 0.75 N - 0.10 Balance Expected Chemical Properties of Parts
systems. The parts built from EOS Stainless Steel 316L can be machined, shot-peened and polished in as-built or stress relieved states if required. This research will use parts that have not been stress relieved. EOS states that the relative density of finished parts, using standard
parameters, are approximately 100% or minimum 7.9 g/cm3 (EOS E-Manufacturing Solutions, 2014a). The expected material composition can be found in Table 2-1, each element shown in percentages, while the measured chemical composition may be found in the appendix. According to EOS (2014a) this chemical composition is within limits of ASTM F138 “Standard
Specification for Wrought 18Cr-14Ni-2.5Mo Stainless Steel Bar and Wire for Surgical Implants” (EOS E-Manufacturing Solutions, 2014a). Also the expected chemical composition of the
purchased parts can be found in Table 2-2.
Kamath (2014) discusses various manufacturing strategies for achieving greater density in 316L stainless steel parts. The strategies investigated here were changing of the scanning parameters of the machine. These parameters included laser power; scaling from 150 to 400W; and adjusting the laser scan speeds. It was found that with a given laser power increasing the scan speeds could result in insufficient melting and a lower part density. As well as when at high laser powers, the density is higher over a wider range of scan speeds, unlike at lower laser powers. Kamath’s experiment showed that when using optimized parameter settings on a machine, it is possible to produce small parts with >99% relative density using SLM (Kamath, El-dasher, Gallegos, King, & Sisto, 2014). When a process uses properly generated process parameters, the balling phenomenon is easily avoided. Along with the possibility of balling, residual stresses in AM produced parts can be a significant setback. According to Mercelis
(2006) residual stresses in parts are not always disadvantageous, sometimes the stresses are induced so that a part contains a certain quality. However, residual stresses are primarily unwanted as they result in a deformation of the intended dimensions. Mercelis (2006) explains the two mechanisms which introduce residual stress as follows:
The first mechanism introducing residual stress is called the temperature gradient mechanism (TGM, Figure 2-2). It results from the large thermal gradients that occur around the laser spot. Owing to the rapid heating of the upper surface by the laser beam and the rather slow heat conduction, a steep temperature gradient develops. Since the expansion of the heated top layer is restricted by the underlying material, elastic compressive strains are induced. When the material’s yield strength is reached, the top layer will be plastically compressed. In absence of mechanical constraints, a counter bending away from the laser beam would be perceived. During cooling the plastically compressed upper layers start shrinking and a bending angle towards the laser beam develops. This mechanism is also present in SLS and SLM, where the underlying layers inhibit the expansion of the heated top layers. It is important to notice that this
mechanism does not require the material to be molten.
A second mechanism that induces residual stresses is the cool-down phase of the molten top layers (in SLM). The latter tend to shrink due to the thermal contraction. This
deformation is again inhibited by the underlying material, thus introducing tensile stress in the added top layer and compressive stress below (Mercelis & Kruth, 2006).
Other research investigating optimal process parameters discusses residual stresses in parts when using varying process parameters. The research of Mercelis (2006) involves 316L stainless steel to determine how residual stresses are affected by changes in the SLM building
process. The results stated that a reduction of residual stresses is possible by heating the build plate as it reduces the temperature gradients during building. It is also discussed that it is possible to reduce the stress levels by applying a heat treatment to the part using the laser, by multiple scans, though no drastic reductions could be obtained in their investigation. A major conclusion was a distinction between parts left on the build plate and parts what were removed. Mercelis (2006) states that parts which remain attached to the build plate contain high amounts of stress levels. While parts which are removed from the plate contain lower stress levels, but those parts suffer from deformation during the part removal (Mercelis & Kruth, 2006).
For the EOS metal systems there are three different Parameter Sets (PS), each are meant to achieve a different attribute, and are as follows:
Speed – (30 – 60 µm layer thickness) – higher productivity, good surface quality. The Speed PS represents a good compromise between building speed and surface quality. The building time is shorter compared to the Performance PS.
Performance – (30 – 40 µm layer thickness) – good surface quality. This parameter set is ideally suited when the focus is good surface quality. Compared to the Surface PS, it
Figure 2-2: TGM inducing residual stress (Mercelis & Kruth, 2006)
offers a higher productivity due to thicker powder layers which helps to reduce production costs.
Surface – (20 µm layer thickness) – fine details, high surface quality. Compared to the above parameter sets, the Surface PS is built with the lowest layer thickness. Therefore, it is the perfect choice for parts that require fine and high detail resolution and best surface quality (EOS e-Manufacturing Solutions, 2013b).
The experimentation with the EOS M290 included the prearranged Performance parameter set, which will provide the best all-around performance. Most process details of the parameter sets provided by EOS are not known, such as the laser power, scan speed, etc. Though some technical data are given such as; each powder layer has a thickness of 20 µm, the typical achievable part accuracy in small parts is approximately ± 20-50 µm, as well as expected surface roughness of as-manufactured parts being R. 13 ± 5 µm; R. 80 ± 20 µm (EOS E-Manufacturing Solutions, 2014a).
Microstructure and Grain Structure from SLM Process
Microstructure of a material can be described as, “The arrangement of phases and defects within a material (Materials and Minerals Science Course C: Microstructure).” Microstructures are generally generated when a material undergoes a phase transformation brought about by change in temperature and/or pressure. An example being the cooling of a melt pool during a SLM process. Solidification of a crystal from a melt occurs through a process of nucleation and growth. Below the melting temperature, small clusters of atoms in the melt come together through random chance to form a small crystalline particle (a nucleus). The nucleus forms a template onto which other atoms can attach. Each nucleus grows into an individual grain of the crystal. When adjacent grains impinge they form grain boundaries. Since individual nuclei form
in different orientations, there is no orientational relationship between adjacent grains (Materials and Minerals Science Course C: Microstructure). These grains and grain boundaries make up the microstructure of a material. During the process of SLM a melt pool is formed in the powdered material as the laser passes over, and as this melt pool cools the microstructure forms. While the microstructure is forming, the melt pool is also adhering to the previously melted layer of the part. This fresh melt pool’s grains interact with that of the previous layer which cause the two layers to bond. In theory, each time these layers bonded together the microstructure should remain uniform, but this is not the case. A ‘phase’ is taken to be any part of a material with a distinct crystal structure and/or chemical composition. Different phases in a material are separated from one another by distinct boundaries (Materials and Minerals Science Course C: Microstructure). It can then be described that each melt pool caused by the laser can be seen as a phase. As SLM is a layered method, and the microstructure for all layers are not uniform, the distinction between the layers can be seen using microscopy. Figure 2-3 allows the various melt
Figure 2-3: Balling characteristics when oxygen=0.1% (Li, Liu, Shi, Wang, & Jiang, 2012)
pools formed during the SLM process to be seen, each running parallel and overlapping with one another.
Effects of Various Orientations
Along with parameter settings, the orientation in which a part is built can be adjusted to provide different results. When describing the orientation of a SLM manufactured part it is necessary to have a coordinate system or terminology in which to describe the orientation.
ASTM standard 52921 provides the standard for identifying the various 3D orientations for parts. This coordinate system uses the X, Y, and Z axes of the build volume origin, where the parts orientation is described by listing which axis is parallel to the longest overall dimension of the
Figure 2-4: Orthogonal Orientation Notation (ASTM ISO / ASTM52921-13,, 2013)
part first, followed by the axes parallel with the second longest dimension, followed by the axis which is parallel to the third longest overall dimension. This will allow part orientations to be described by XYZ notations as shown in Figure 2-4. Orthogonal orientation notation may be abbreviated where symmetry allows, thus when using flat tensile test coupons bilateral symmetry can be applied allowing the notation to be shortened to ZX, or XY as shown in Figure 2-5.
Simonelli (2014) looked at what effect build orientation had on SLM created parts in Ti-6Al-4V. The experiment looked at three orientations of tensile coupons, these being ZX
(vertical), XY (flat), and XZ (edge). The flat orientation of these parts showed significant curling during the SLM process. Some specimens were curled enough to be discarded, while others were machined into flat parts. The results from the tensile testing showed the elastic modulus did not vary with the change in the build orientation. The flat oriented tensile bars gave the lowest elongation at failure. This result was attributed to the curling of the parts, thus preventing an even powder deposition when forming layers. Simonelli stated that the edge oriented bars
Figure 2-5: Example of Symmetry Abbreviation of Orthogonal Orientation Notation (ASTM ISO / ASTM52921-13,, 2013)
produced the best tensile properties and the greatest elongation at fracture (Simonelli, Yse, & Tuck, 2014).
Tolosa (2010) conducted an experiment to see the effects on AM created parts with various build orientations and angles. These parts used AISI 316L stainless steel. The various orientations were displayed as case A, B, and C; where case A samples were manufactured in the XY orientation; case B were built in the XZ orientation; case C in the ZX orientation; and case D was built in the ZX with various angles with respect to the build plate. Within each class
different groups of parts were built with different angles rotating about the Z axis. It should also be noted that to avoid the use of supports from the samples to the build plate, the samples were built with prismatic geometry and then machined to size after the AM process completed. Tensile tests were performed on both the SLM manufactured specimens and parts created with traditional manufacturing, in this case rolled steel machined to size. When Tolosa compared the results of the various cases for orientation, for strength the best option is the case A (XY)
orientation. While case C provides the best ductility values (Tolosa, Garciandía, Zubiri, Zapirain, & Esnaola, 2010).
Much research on SLM capabilities involve Ti-6Al-4V and 316L stainless steel, Mertens (2014) states it is because of the materials use in biomedical and aeronautical applications. Mertens performed an experiment which involved both these materials. The goal of this experimentation was to see how the SLM process effected mechanical properties of the two materials, with different build orientations seen in Figure 2-6. Uniaxial tensile tests were
performed to samples of both materials in accordance with the ISO 6892-1 B 25: 2009 standard. An optical micrograph of 316L showed semi-circular shapes perpendicular to the building direction, which corresponded with individual melt pools. Though two different types of
porosities could be observed. Of these were spherical pores formed by gas bubbles between melt pools, and larger more elongated shapes localized between melt pools of two successive layers. These larger defects were scarce in the OY and OX orientations, however a greater number were found in the OZ orientation. These elongated shapes can be attributed to unmelted powder or insufficient remelting of the previous layer of material. After tensile testing it was found that the OX and OY orientations had similar material properties as well as a typical ductile fracture behavior. Though the OZ orientation specimens produced much lower strength results as well as much smaller elongation during testing. The reduced material properties for the OZ orientation can be attributed to the defects caused by lack of melting. Mertens concluded by comparing the two materials to each other. Fro0m this it was determined that Ti-6Al-4V is more susceptible to the build-up of internal stresses than 316L. Though material defects as a result of the SLM process appear more often in the 316L stainless, this was found to correspond with the difference in thermal conductivity of the two materials (Mertens, et al., 2014).
Figure 2-6: Representation of various orientations of tensile samples with respect to building direction (oz)
EOS Machine Specifics
With the SLM process many experiments and evaluations have been formed using a wide variety of different brands of machines and processes. Through this investigation only a few research studies were conducted using EOS SLM systems. Most of the research briefly discuss the M290 system’s capabilities or use it to determine possibilities with AM processes.
Bhavar (2014) reviews the present capabilities and challenges of AM systems. This review also compares various types of systems such as SLM, SLS, and EBM, to discover advantages, disadvantages, as well as differences in capabilities and materials. Within the discussion is also included a variety of systems available on the market including different EOS systems, but specifically the comparison contains the EOS M290 SLM system. The author primarily discusses the possibilities and applications possible, and some challenges with AM, and further compares specifically of the SLM and EBM systems. These two systems have a major difference in the laser type they use, but also in how the powder bed is heated during building. SLM systems heat the build plate to a wanted temperature and let the heat travel through the part being built, where EBM preheats the actual powder layer about to be scanned. Also the heating temperatures are vastly different, where the EOS M290 system heats the plate to 85°C and the EBM system heats the powder layer to around 700-900°C. Also the supports needed for EBM are needed for head conduction rather than part support. EBM systems have a higher build rate compared to the SLM, but also inferior dimensional and surface finish qualities. EBM systems also build within a vacuum, which is necessary for the quality of the electron beam, as well as reducing thermal gradients and possible oxidation of the parts like titanium alloys. Even with EBM systems having these advantages SLM is still more popular. Bhavar attributes this popularity to EBM
systems having higher machine cost, low accuracy and small build volumes (Bhavar, et al., 2014).
The EOS M290 system can also be found in the work of Krantz (2015) where a model was built to discover the viability of full scale production using AM versus traditional
manufacturing, including milling and die casting. While creating the cost estimation model it was discovered that as needed accuracy in a part increased, the price for milling also increased and was not a linear change. This resulted in a step away from exact prices and towards price-spans. This work did result in a working mathematical model for each process, but was not used to specify which process at the time which method was more cost efficient (Krantz & Sjöö, 2015).
Again using the EOS M290 system Poyraz (2015) performs an investigation of block support structures of overhanging geometry parallel to the XY plane during the building process. The first part of the experimentation investigated the impact of the support dimensions, such as hatch distance of a block. However, the second set of experiments focused mainly on the effects of part to support contact in the way of teeth dimensions. The two experiments were controlled by dimensional inspection and light optical microscopy. Each experiment was performed using Inconel 625, and constant process parameters to avoid introducing different variables. The results of change in hatch distance showed when the hatch distance was increased the overhanging geometry was more distorted and at the max, one mm, distance the separation between the part and support structure was most significant. Thus keeping a smaller hatch distance will cause the part to distort less as it is better connected to the support structure. For the change in tooth
dimensions it was found both the top length and Z offset value reductions influence the distortion results. However, it was also observed that when the top length; the length of the tooth touching
the part; increases, the impact of the Z offset; the height of the tooth; value decreases. In a final conclusion Poyraz states that with regard to part distortion and overhang geometry lifting, hatch distance has a more significant effect when changed. This experiment found that using lower hatch distance is useful for maintaining less distortion of parts, and the best results were achieved with a 0.5mm hatch distance (Poyraz, Yasa, Akbulut, Orhangül, & Pilatin, 2015).
Tensile Properties/Test Stress Risers
When discussing stress concentrations concerning AM processes, it usually pertains to uncontrolled or unwanted features that form during the building process are historically the primary factors. This can vary from a part detaching and curling during the build, to portions of the powder layer not completely melting and creating larger than normal porosity defects. At the time of this research no testing has been found in the area of purposefully forming a stress concentration, such as a hole, in a part created by SLM meant for tensile testing to determine mechanical properties.
Research has been done in the area of tensile testing specimens which contain a stress concentration in the form of a circular hole. Most of this research has been in the area of
mathematical models and estimating how the specimen will react during testing. There was little information found on testing materials with this type of stress concentration and the research performed using metals was done using large sheet type specimens that were multi-axially loaded. An example of the desired tensile specimen geometry may be seen in Figure 2-7. As stated, there has been no research found using this specimen geometry within metals.
Standard for Tensile Testing Metals
ASTM E8/E8M – 13a is the standard for test methods for tensile testing of metallic materials, and will drive the tensile testing performed in this experimentation. The specific size and geometry for the test specimen may be found in Figure 3-1. This test will be using
rectangular tension test specimens. The following are sections necessary for set-up processes and predetermining test settings pertaining to this experiment.
Zeroing of the Testing Machine: The testing machine shall be set up in such a manner
that zero force indication signifies a state of zero force on the specimen. Any force (or preload) imparted by the gripping of the specimen must be indicated by the force measuring system unless the preload is physically removed prior to testing. Artificial methods of removing the preload on the specimen, such as tearing it out by a zero adjust pot or removing it mathematically by software, are prohibited because these would affect the accuracy of the test results.
Figure 2-7: Tensile specimen containing a circular hole stress concentration
Gripping of the Test Specimen: For specimens with reduced sections, gripping of the
specimen shall be restricted to the grip section, because gripping in the reduced section or in the fillet can significantly affect test results.
Speed of Testing: Speed of testing may be defined in terms of (a) rate of straining of the
specimen, (b) rate of stressing of the specimen, (c) crosshead speed, (d) the elapsed time for completing part or all of the test, or (e) free-running crosshead speed.
Crosshead Speed: the allowable limits for crosshead speed, during a test, may be
specified in mm/min in this case. Many testing machines are equipped with pacing or indicating devices for the measurement and control of the crosshead speed during a test, but in the absence of such devices the average crosshead speed can be experimentally determined by using suitable length-measuring and timing devices.
It is from this standard that the testing procedures and tensile specimen geometry have been determined.
CHAPTER THREE: METHODOLOGY
The methodology of this research covers each step that was taken in preparation of the parts for each production method, and the tensile testing and data recording of each part from each production method.
All test specimens used in this experiment have been created to the size and shape recommended by the ASTM E8 standard test methods for tension testing of metallic materials. The chart containing the recommended sizing can be found in Figure 3-1. The specimens use the measurements of the sheet type, 12.5 mm wide selection. Along with these measurements a
Figure 3-1: Rectangular Tension Test Specimens (ASTM E8 / E8M-15a, 2015)
thickness of 3.175 mm was used. Both methods of part manufacturing will be aiming for these measurements. All actual measurements of parts were taken and recorded for later use. The machined specimens were purchased from Lab Testing Inc., who manufacture and test various specimens. The specimens were purchased in an untested state so that the machined and AM specimens were tested using the same equipment in the same conditions.
Part position and Support Structure
The part was first designed using Pro Engineer, using the dimensions determined by the standard. Both geometries, with and without the stress concentration were modeled. These 3D models were then converted to STL files to be used with other software. These STL files were then transferred to Magics, which is a popular software used by many AM processes. This software was then used to generate the 3D model in a space where support structure could then be formed. Magics generates support structure on parts where it believes it will be needed during the SLM process. On many parts it is formed on the underside or overhanging geometries to ensure the part is fully supported during processing, to prevent the parts from curling or dipping which could result in a failed build. It is then possible to remove areas of suggested support structure or to add more if necessary. This allows for any unwanted or unnecessary support to be removed, which is primarily done to avoid the need for more post processing.
Support structure was created for each geometry, as each had various requirements. All geometries used block support, except the stress concentration in the edge orientation, which used gusset supports. For the flat specimens, the solid geometry required support material beneath the entire part, shown in Figure 3-2. Whereas for the part containing the stress
concentration, no support structure was created where the hole exists, as seen in Figure 3-3. The differences in necessary support structure may also be seen in the differing support structures for parts built on edge. For example in the edge oriented test specimen instead of removing
unnecessary support structure, more was needed to be used within the stress concentration. Along with the support structure needed directly below the part, it is seen in Figure 3-4 that when the stress concentration is being formed in this orientation it is necessary to support it, as the top half of the arc acts as an overhanging geometry. If the support structure was not being used in the stress concentration the resulting shape would not resemble what was wanted. This is because, as overhanging material is being scanned it has a tendency to curl upwards due to heat and residual
stresses. When this layer curls, the next layer is scanned at this raised position, and thus causing a change to the desired shape. As a result of this, the stress concentration more resembled a tear drop shape rather than a circular hole. An example of this may be seen in Figure 3-5.
Once the specimens and their respective support structure was generated, the parts were moved to EOSPRINT, where the layout of the build plate was designed. In EOSPRINT it is possible to visually position the desired parts within the build volume. This is done to be sure the parts fit but also to optimally position the parts for processing. The need for positioning of the parts depends on the part geometry, as well as preventing possibilities of failure during the build.
Figure 3-4: Edge oriented test specimen showing supported stress concentration
Figure 3-5: Edge oriented test specimen build without stress concentration supports
When creating the build plate for these testing specimens care was taken to avoid possible issues with part positioning. Some of these being staggering the parts with relation to the recoating blade seen in Figure 3-6. There could be a greater chance of the blade catching the edge of the parts if they were all aligned square with the blade. Another part positioning which was taken into consideration was the part angle with respect to the edges of the build plate. Parts were rotated to angles around 10°. This was again done to avoid having square contact with the recoating blade. These precautions were again taken as there is a possibility the recoater blade will catch on edges flat with the blade. Both of these position adjustments can be seen in Figure 3-6. Once the support structures have been generated, and the layout of the build plate has been created, the file is then transferred to the M290. Within the transfer process the build is broken down into layers and sent to the machine in this format.
Once the code was transferred to the machine, the machine itself need to be prepared for operation. There are a set of steps that must be taken before a build may be started. The first step is loading the build plate into the machine, once seated in place the build plate is heated to a required temperature. The M290 requires the build plate be at 80°C before the build may be started. Once the plate reaches the required temperature the bolts are put in place and tightened, keeping the plate in place during the building process. Now that the plate is in place, the first layer must be made. This is done by first leveling the plate in both the X and Y directions with respect to the recoater blade. This is done by sliding spacer gages between the recoater blade and the build plate. It is first done with the recoater blade in the left half of the build plate, adjusting the plate to be level for the front and back halves of the plate. The recoater blade is then moved to the right half of the plate and adjusted so that the left and right halves of the build plate are level. This leveling is then checked by manually placing the first layer, by moving the recoater blade across the build plate while spreading a layer of the powdered metal to be sure the resulting layer is evenly spread. This layer does not have to be an exact thickness, as it is being created by hand, but is usually between 20-40µm thick.
After a layer of acceptable thickness has been made, and the plate is confirmed to be level with the recoater blade, the rest of the machine preparation must be made. Once the build volume door has been completely closed, the build volume’s atmospheric requirements must be met. These are steps that are done at the same time. Both the build volume and the machines filtration system must be purged by an argon or nitrogen atmosphere to reach a certain oxygen percentage. An argon atmosphere is needed to use the 316L stainless steel material. The required oxygen percentage in the build volume and filtration system are 0.1% and 1.0% respectively.
Once this step is complete, the machine has been fully prepared for operation. The loaded build plate code is started and the machine builds the parts. The actual building of the parts varies depending mostly upon the geometries being created, ranging anywhere from 8 hours to 120 hours for particularly large builds. It is a rule of thumb that the taller the part the longer the build will be, but it can be presumed that the more volume required to create, the longer the build will take to complete.
Preparation of Printed Pieces
After the machine has finished scanning the final layer of the build and has finished, the parts must be removed from the build volume. As the machine scans each layer of the part, and lays a new layer of powder, the entire build plate area is covered. This continues through the entire process, and as a result the parts are encased in the excess powdered metal, seen in Figure 3-7. This powder must then be transferred and sieved to be used again. Once the entirety of the powder has been removed and the parts have been vacuumed of powder, the bolts are removed and the plate can be taken out. When the build plate exits the building chamber, the part is fully manufactured, though there are still several steps needed before the part is usable. To begin the post processing, the parts must first be removed from the build plate. This can be accomplished many ways, a wire EDM can be used for this instance, though in this case a horizontal band saw will be used. Another reason that support structure is used in most manufactured parts is to assist in the removal of the part. This support structure not only creates the teeth geometry for easier removal, but also gives material between the build plate and the part itself for a cutting device. Because of this, neither the part nor the build plate are damaged during the part removal. For the
parts used here a band saw is used to remove the parts from the plate. Care must be taken here as to not damage the plate with the blade, but the blade needs to be close enough to the plate as to not cut into any parts but rather only the support structure. After being removed from the plate each part must have the support structure removed.
This part of post processing can change methods based on the geometry and where the supports are being removed. There are a variety of methods used for removing support structure, such as a CNC mill or lathe, grinding/sanding station, or removal by hand. Because the nature of the process of SLM is based on increased temperature of the material, raising the temperature during post processing was avoided where possible during this experimentation. This meant that any tooling was circumvented and a simpler process was used. Each of the individual specimens had their support structure removed by hand, using a hammer and chisel. This was made easier due to the teeth of the support structure at the base of the specimen. These teeth may be seen in Figure 3-8, where the bottom “dashed” area is the support structure. The chisel was aligned with the teeth of the support structure when struck by the hammer. As the teeth and support structure
was hatched and not a fully dense part, it gave way easier than the part itself would have, allowing the chisel to follow the edge of the part only removing the support structure. This allowed for easy separation from the part. Because of the method used to remove support structure, the specimens were left with a rough surface finish where the support structure was removed. These surfaces were filed, using a metal file, to remove the roughness which could have possibly been remaining tooth and support structure. This method was used for each geometry to remove the support structure spanning from the part to the build plate. As shown in Figure 3-4, the edge oriented SLM specimen containing the circular stress concentration required gusset support structure to properly form the circular shape. This support structure was also removed though a different approach was used. Instead of using a tool to cut out the support material, a small circular metal file was used to remove the support material. As gusset supports are made up of a fin like geometry there was not much material to remove. The holes were filed out until the correct corresponding size was achieved. After the removal of support structure the parts were able to be tested.